Presentation on theme: "GUIDE FOR CONSTRUCTION OF GROUND-SUPPORTED CONCRETE SLABS USING: Factory Floor Slab, Bristol. England. Recycling Center at Debabarrena - San Sebastian,"— Presentation transcript:
GUIDE FOR CONSTRUCTION OF GROUND-SUPPORTED CONCRETE SLABS USING: Factory Floor Slab, Bristol. England. Recycling Center at Debabarrena - San Sebastian, Spain Valencia Train Station, Spain Replacing Traditional Steel Mesh
All data included in this guide relates exclusively to the use of Fibratec V12-AM Alkali- Resistant Glass Fibre. This fibre complies with BS EN 15422 : 2008 : Precast Concrete Products – Specification of Glass Fibres for Reinforcement of Mortars & Concretes and has the highest Zirconia content of all ARG Fibres. This provides resistance to alkalis present in the concrete mix. All recommendations within this guide are from extensive testing and evaluation by the Structures Department of University of Almunia de Doña Godina (EUPLA) in Zaragoza, Spain. INDUSTRIAL AND VEHICULAR FLOORS The following procedure will assist with the slab design : STEP1: Ascertain the bearing rate of the substrate. (Typically expressed as CBR (California Bearing Ratio) percentage (%) or “k” factor) STEP2: Determine the application of the concrete slab : Eg Car park, truck park, industrial warehouse floor. Presence of racking, forklifts etc. This information is important to determine the contact area of loads on the concrete slab. STEP3: Identify the concrete grade, Eg C25, C30 etc. STEP4: Select the correct slab thickness with fibre concrete to allow for punching shear and flexural strength for the given loads. IMPRINTED OR POLISHED PEDESTRIAN FLOORS (Pavements, Recreation Areas etc) We recommend a dosage of between 1-2 kg of FIBRATEC V12-AM per cubic metre of concrete. Fibratec fibres reduce cracking and and provide reinforcement. Fibratec fibres distribute 100% evenly thoughout the slab. Fibratec fibres are invisible at the surface. Fibratec fibres are ideal for imprinted or polished concrete finishes. Fibratec is compatible with all chemical additives and concrete admixtures. IMPORTANT INFORMATION! By following these four steps and our recommendations, most ground- supported concrete slabs may be constructed using Fibratec V12-AM. This removes the requirement for costly labour involved in transporting, cutting and placing of traditional crack-control, steel mesh.
Converting bearing rate or “k” value of the ground to CBR : Ev₂ MN/m² “k” value Bearing Rate MpakPa/mmN/mm³T/m³% CBR 30250,025 2.5003,0% 60500,05 5.0008,0% 1201000,1 10.00038,0% In the absence of ground conditions, we advise that the substrate should be compacted as much as possible. Assume a 3% CBR value in order to provide a sufficient safety margin. STEP 1 COMPLETED: “CBR” OF THE SUBSTRATE ESTABLISHED CBR STEP 1 IDENTIFY THE BEARING RATE OF THE SUBSTRATE (% CBR) EXPECTED CBR ASTM SOIL CLASIFICATIONDESIGNATIONDESCRIPCTION NOT COMPACTED COMPACTED Coarse grained soils more than 50% retained on or above No.200 (0.075 mm) sieve Gravel > 50% of coarse fraction retained on No. 4 (4.75 mm) sieve Clean gravel <5% smaller than #200 Sieve GW Well-graded gravel, fine to coarse gravel OVER 38% GP Poorly graded gravel OVER 38% Gravel with >12% fines GM Silty gravel OVER 20% GC Clay gravel OVER 20% Sand ≥ 50% of coarse fraction passes No.4 sieve Clean sand SW Well-graded sand, fine to coarse sand OVER 20% SP Poorly graded sand OVER 20% Sand with >12% fines SM Silty sand OVER 20% SC Clay sand 15% Fine grained soils 50% or more passing the No.200 sieve Silt and clay liquid limit < 50 ML Inorganic silt5%10-15% CL Inorganic clay of low plasticity, lean clay5%10-15% OL Organic silt, organic clay4%6% Silt and clay liquid limit ≥ 50 MH Inorganic silt of high plasticity, elastic silt4%6% CH Inorganic clay of high plasticity, fat clay3%4% OH Organic clay, organic silt3%4% PT Peat00
STEP 2 DEFINE THE APPLICATION OF THE SLAB IN ORDER TO IDENTIFY THE AREA OF CONTACT BETWEEN LOADS AND THE CONCRETE SLAB TYPE OF CONSTRUCTIONTYPE OF APPLICATION Defined contact area (cm ) INDUSTRIAL AREA Storage racks/small forklift 11X11 Truck / trailer 40X40 Small or big forklift 15X15 PARKING/TRANSIT AREA OR ACCESS FOR: Cars 15X15 Vans 20X20 Trucks, trailers 40X40 CONTACT AREA In the absence of reliable information regarding the intended use of the concrete slab, or to allow for future change of use, we recommend the use of the smallest defined contact area (11cm x 11cm) in order to provide a safety margin. STEP 2 COMPLETED: THE CONTACT AREA WITH THE SLAB IS DEFINED STEP 3 DEFINE THE CONCRETE GRADE FOR THE CONCRETE SLAB. TYPICAL GRADES OF CONCRETE FOR FLOOR SLABS ARE C25 OR C30. For site mixed concrete, using a small mixer, we suggest the following procedure for proportioning materials an approximate grade of C25 (Note : when using volumentric proportions the compressive strength should always be confirmed by testing/proportions modified to suit available materials) Using this guide, Point Load Values from the C25 column would be used in STEP 4. BY WEIGHT (For 100 lt of concrete) CEMENT: 28 kg SAND: 70 kg AGGREGATES (12-20mm) 125 kg WATER: 16 kg STEP 3 COMPLETED: CONCRETE GRADE CEMENTSAND 1 full container2 full containers + 1/3 container AGGREGATES (12-20 mm) 3 full containers WATER 1/2 container + + + BY VOLUME (Using the same size container)
STEP 4 CALCULATING THE THICKNESS OF THE SLAB, BASED ON THE FLEXURAL AND PUNCHING STRENGTH OF A GIVEN GRADE OF FIBRE-ENTRAINED CONCRETE. SECURITY FACTOR S: γ G =1,35 (own weight), γ Q =1,50 (overload) and γ c =1,50 (concrete) SUPPORTED POINT LOADS WITH USE OF 3 KG OF FIBRATEC V12-AM / M³ OF CONCRETE AREA OF CONTACT WITH SLAB: 11CM X 11CM (footprint of point load) Typical application : Small forklifts with small wheels, storage racks in warehouse… SUPPORTED POINT LOADS WITH USE OF 3 KG OF FIBRATEC V12-AM / M³ OF CONCRETE AREA OF CONTACT WITH SLAB: 15CM X 15CM (footprint of point load) Typical application : Car park, large-wheeled forklift… SLAB THICKNESS (cm) CBR 3% - 8% - 38% Distance between expansion joints INDOOR SLABS Distance between expansion joints OUTDOOR SLABS Depth of cut joint (cm) C25 * kg point load C30 * kg point load 12210022003m – 3.5m2m - 3m4 13240025503m – 3.5m2m - 3m4 14270029003.5m - 4m2.5m – 3.5m4.5 15300032003.75m – 4.5m3.5m - 4m5 16340036003.75m – 4.5m3.5m - 4m5 17380040004m - 5m3.5m - 4m5.5 18410043504m - 5m3.5m - 4m6 19450047504.25m – 5.50m4m - 5m6 20490052004.25m – 5.50m4m - 5m6.5 21530057004.5m - 6m4m - 5m7 22575062004.5m - 6m 7 23635067004.75m – 6.5m4.5m - 6m7.5 24675071504.75m – 6.5m4.5m - 6m8 SLAB THICKNESS (cm) CBR 3% - 8% - 38% Distance between expansion joints INDOOR SLABS Distance between expansion joints OUTDOOR SLABS Depth of cut joint (cm) C25 * kg point load C30 * kg point load 12238025003m – 3.5m2m - 3m4 13280029003m – 3.5m2m - 3m4 14300032003.5m - 4m2.5m – 3.5m4.5 15340035803.75m – 4.5m3.5m - 4m5 16370040003.75m – 4.5m3.5m - 4m5 17410044004m - 5m3.5m - 4m5.5 18450048004m - 5m3.5m - 4m6 19490052004.25m – 5.50m4m - 5m6 20530056504.25m – 5.50m4m - 5m6.5 21580061004.5m - 6m4m - 5m7 22620066004.5m - 6m 7 23670071004.75m – 6.5m4.5m - 6m7.5 24720077004.75m – 6.5m4.5m - 6m8 Length of cut joint should not be greater than = width x 1,5. Square cuts are advisable For 2 kg dose of V12-AM Fibratec /m³, simply decrease point loads given in above table by approximately 10% Note that for small load contact areas iqual or smaller than 20 x 20 cm, flexural strength is not as important as punching (puntural) strength of concrete,. Therefore, bearing rate CBR does not influence the load supported by the slab. Length of cut joint should not be bigger than = width x 1,5. Square cuts are ideal * For 2 kg dose of V12-AM Fibratec /m³, simply decrease point loads given in above table about 10%
SUPPORTED POINT LOADS WITH USE OF 3 KG OF FIBRATEC V12-AM / M³ OF CONCRETE AREA OF CONTACT WITH SLAB: 20CM X 20CM (footprint of point load) Typical application : Car Parking, small trucks, larger forklifts SLAB THICKNESS (cm) CBR 3% SLAB THICKNESS (cm) CBR 8% SLAB THICKNESS (cm) CBR 38% C 25 *kg point load C 30 *kg point load C 25 *kg point load C 30 *kg point load C 25 *kg point load C 30 *kg point load 12 35003600 12 40004100 12 40204150 13 39004000 13 43504400 13 44504500 14 41504250 14 47004800 14 48504900 15 46004750 15 49005000 15 51005200 16 49505050 16 53005400 16 56005700 17 52005400 17 56005800 17 60006200 18 58005900 18 60006100 18 65506800 19 61506300 19 64006650 19 72507500 20 68006900 20 70007400 20 78508340 21 73507550 21 79508400 21 84008950 22 81008400 22 80009400 22 90009500 23 90009300 23 955010100 23 955010100 24 980010100 24 1010010800 24 1010010800 SUPPORTED POINT LOADS WITH USE OF 3 KG OF FIBRATEC V12-AM / M³ OF CONCRETE AREA OF CONTACT WITH SLAB: 40CM X 40CM (footprint of point load) Typical application : : Truck parking, truck or trailer with multiple axles, transit areas… SLAB THICKNESS (cm) CBR 3% - 8% - 38% Distance between expansion cut joints INDOOR SLABS Distance between expansion cut joints OUTDOOR SLABS Depth of cut joint (cm) C 25 * kg point load C 30 * kg point load 12260028503m – 3.5m2m - 3m4 13300032003m – 3.5m2m - 3m4 14340036003.5m - 4m2.5m – 3.5m4.5 15380040003.75m – 4.5m3.5m - 4m5 16410044003.75m – 4.5m3.5m - 4m5 17450048004m - 5m3.5m - 4m5.5 18495052004m - 5m3.5m - 4m6 19540058004.25m – 5.50m4m - 5m6 20580061804.25m – 5.50m4m - 5m6.5 21630067004.5m - 6m4m - 5m7 22680072504.5m - 6m 7 23735078004.75m – 6.5m4.5m - 6m7.5 24785082504.75m – 6.5m4.5m - 6m8 Information regarding distances between cut joints for above table is exactly the same as indicated in the above tables. Please check slab thcikness in previous tables and apply same joint distances and depths when executing your project. NOTE: In small areas of contact up to 20 x 20 cm, flexural strength has less influence than punching shear resistance of concrete indetermining the limit loads. For this reason, the CBR is not the primari influence. Length of cut joint should not be greater than = width x 1.5. Square cuts are advisable For 2 kg dosage of V12-AM Fibratec /m³, simply decrease point loads given in the above table by approximately 10% Length of cut joint should not be greater than = width x 1.5. Square cuts are advisable. For 2 kg dose of V12-AM Fibratec /m³, simply decrease point loads given in the above table by approximately 10%
GENERAL RECOMENDATIONS Expansion cracks can generally be avoided by making cut joints and following the following recommendations. Regardless of the use of traditional mesh or fibre-entrained concrete, these practices are essential in order to ensure the highest quality of construction. Using fibres does not remove the need for good concrete construction practice. Fibres only replace traditional steel mesh. Cover the ground with a polyethylene sheet before pouring concrete. Constantly irrigate, cover the slab surface with polythene or apply a curing compound during first 7 days after pouring concrete. This controls the temperature and humidity in order to cure the concrete, minimising cracks, surface dusting and maximising potential strength. (Especially in areas with sun or wind exposure) As a general recommendation, cut construction joints during the first 24 hours after pouring concrete. Distances between cuts and depth of cuts are exactly the same as normal concrete slab construction. Avoid internal angles smaller than 60° which will increase the liklihood of cracks. When pouring concrete over existing concrete, clean the surface and apply a recommended bonding layer. For vehicle parking areas the minimum slab thickness should be 8 cm. (Maximum aggregate size = 20mm). Do not exceed 15 m between working joints. Concrete slabs should not be poured under 0°C or over 40°C ambient temperatures, without adequate protection. 5 m 2 m WRONG 3 m CORRECT 2 m Incorrectratio between length and width WRONG Smaler angle than 60 ° WRONG Staggered cuts 25m 10 m CORRECTWRONG Placing water manholes, columns and other rigid elements CORRECTWRONGCORRECT WRONG For road traffic areas construct cut joints with dowel joints, following these recommendations: Fibrated C25 or C30 concrete slab Polyethylene sheet thickness 0.2 mm 1 or 2 layers Cut joint (retraction) Gravel leyer Either smooth or plastic covered bars to allow horizontal movement, placed each 30 cm. Column Cut width 3-4 mm Polyspan plate of 10 mm in all perimeters Detail of cut joints for water manholes, Columns and very rigid elements: CORRECT WRONG DOWEL JOINTS Slab Thickness Bar Length Bar Diameter cm 12 to 18402 18 to 30502.5 When cut in diamond shape, minimum distance from column to joint must be 10 cm Placing water manholes, columns and other rigid elements Placing water manholes, columns and other rigid elements Placing water manholes, columns and other rigid elements